Acta Mater 57 (2009) 559 Investigation Of The Indentation Size Effect
Available online at www.sciencedirect.com
Acta Materialia 57 (2009) 559–569
Investigation of the indentation size eﬀect through the measurement
of the geometrically necessary dislocations beneath small indents
of diﬀerent depths using EBSD tomography
Eralp Demir *, Dierk Raabe, Nader Zaafarani, Stefan Zaeﬀerer
Max-Planck-Institut fur Eisenforschung, 40237 Dusseldorf, Germany
Received 11 June 2008; received in revised form 27 September 2008; accepted 27 September 2008
Available online 24 October 2008
We study the link between the indentation size eﬀect and the density of geometrically necessary dislocations (GNDs) through the follow-
ing approach: four indents of diﬀerent depth and hardness were placed in a Cu single crystal using a conical indenter with a spherical tip. The
deformation-induced lattice rotations below the indents were monitored via a three-dimensional electron backscattering diﬀraction method
with a step size of 50 nm. From these data we calculated the ﬁrst-order gradients of strain and the GND densities below the indents. This
approach allowed us to quantify both the mechanical parameters (depth, hardness) and the lattice defects (GNDs) that are believed to be
responsible for the indentation size eﬀect. We ﬁnd that the GND density does not increase with decreasing indentation depth but rather drops
instead. More precisely, while the hardness increases from 2.08 GPa for the largest indent (1230 nm depth) to 2.45 GPa for the smallest one
(460 nm depth) the GND density decreases from %2.34 Â 1015 mÀ2 (largest indent) to %1.85 Â 1015 mÀ2 (smallest indent).
Crown Copyright Ó 2008 Published by Elsevier Ltd on behalf of Acta Materialia. All rights reserved.
Keywords: GND; Size eﬀect; 3-D EBSD; Orientation gradient
1. Introduction The average spacing between immobile dislocations,
which is inversely proportional to the square root of the
Advances in microtechnology require better understand- dislocation density, determines the yield strength of the
ing of materials at small scales. This includes mechanical material . Introduction of additional dislocations such
characterization at small dimensions using methods such as GNDs thus increases the ﬂow strength of the material
as nanoindentation. In this context it was observed that a by reducing the mean spacing between dislocations:
material’s resistance to plastic ﬂow depends on the size of qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
the sample [1,2] and on the deformed volume [3,4]. These sa ¼ cGb qa þ qa
gnd ssd ð1Þ
phenomena are referred to as mechanical size eﬀects.
where c is a geometrical constant ranging between 0.5 to 1,
Physically based models attribute strengthening at small
G is the shear modulus, b is the magnitude of the Burgers
dimensions to the existence of immobile dislocations of two
vector, and qa and sa are the dislocation density and yield
types: geometrically necessary dislocations (GNDs) and
strength on slip system ‘‘a”, respectively.
statistically stored dislocations (SSDs). GNDs provide
GNDs that create rotational gradients of strain are used
the lattice continuity in the presence of curvature [5–8],
to explain size-dependent plasticity at small dimensions
whereas SSDs evolve through random interactions among
[11–15]. For instance, the increase in strength with a
dislocations with plastic strain [9,10].
decrease in diameter of copper torsion wires was attributed
to strain gradients. Ashby and Fleck introduced a material
Corresponding author. Tel.: +49 211 6792 324. length scale parameter that is coupled to the rotational gra-
E-mail address: email@example.com (E. Demir). dients of strain . Later, Fleck and Hutchinson applied
1359-6454/$34.00 Crown Copyright Ó 2008 Published by Elsevier Ltd on behalf of Acta Materialia. All rights reserved.
560 E. Demir et al. / Acta Materialia 57 (2009) 559–569
additional length scale parameters to stretch gradients in normal in the crystal, Eq. (3).1 The same equality holds
order to capture size eﬀects during nanoindentation . when displacements are calculated in terms of gradients
Nix and Gao introduced a physically based intrinsic length in a reference frame.
scale assuming a uniform distribution of GNDs below I I
indents [16,17]. The relative contribution of this eﬀect to dui ¼ bij dxj ¼ 0 ð3Þ
the overall resistance of a material to plastic ﬂow becomes
particularly visible in the nanometer regime . The displacement gradient or distortion tensor, bij, con-
The crystallographic misorientation between two neigh- sists of an elastic and a plastic part, Eq. (4). Additive
boring points can be used as an approximate measure for decomposition of distortion allows the use of either the
the GNDs as shown below in Eq. (2), where qgnd is the elastic distortion, bel , or the plastic distortion, bpl , as a
GND density that is required to accommodate a curvature measure of incompatibility.
x [19,20,28]: dui
x bij ¼ ¼ bel þ bpl
ij ij ð4Þ
qgnd ¼ ð2Þ dxj
Using the elastic distortion as a measure of incompati-
Parks calculated the GNDs by minimizing their total bility in conjunction with Stoke’s theorem, the dislocation
length for diﬀerent possible geometrical arrangements tensor can be obtained from the curl ($Â) of the elastic dis-
[21,22] in face-centered cubic (fcc) crystals. Sun and Rollett tortion, Eq. (5). Elastic distortion consists of both an elas-
applied this method to orientation maps obtained via elec- tic stretch, el, and a rotation, g. This is shown in Eq. (6)
tron backscattering diﬀraction (EBSD) from cross-sections where ‘‘e” indicates the permutation symbol. Ignoring the
of deformed crystals [23–25]. They used the misorientations elastic stretch, the rotational gradients are used to identify
to identify the GND density. the components of the dislocation tensor, a, Eq. (7).
An appropriate selection of the EBSD step size is a crit-
ical issue for the calculation of GND densities. EBSD stud- a ¼ r Â bel ð5Þ
ies on deformed crystals have demonstrated the eﬀect of the api ¼ epkj ðel
ij;k þ gij;k Þ ð6Þ
step size on the accuracy of measured misorientations
api ¼ epkj gij;k ð7Þ
[26,27]. The noise in an EBSD analysis strongly depends
on the step size, the type of deformation and the amount The misorientation, D/, between two points is used to
of strain. On the other hand, the step size determines the calculate orientation gradients, gij,k. In the following we
resolution for a Frank loop analysis . Hence, the step explain the procedure for two arbitrary points with given
size used for the GND analysis has to be low enough to orientations /(1) and /(2). The 24 crystal symmetry opera-
be of microscopic relevance and high enough to ﬁlter out tors (Ocry ) are applied to both orientations to identify the
noise. minimum misorientation.
The size dependence of indentation hardness has been
jD/j ¼ minfcosÀ1 ftr½ðOcry /ð1Þ Þ/T Ocry gg
i ð2Þ j
associated with strain gradients which are realized in the
lattice through GNDs. This motivated us to directly mea- i ¼ 1 . . . 24; j ¼ 1 . . . 24 ð8Þ
sure lattice rotations below indents with the aim of quanti- D/ ¼ /ð2Þ /À1 ð9Þ
fying the density of these defects. Monitoring the evolution
of lattice rotations, GND densities and hardness in the The orientation diﬀerence between the two points is esti-
same set of experiments may help to better understand mated in terms of Eq. (10) where I is the second-order iden-
indentation size eﬀects. For this purpose we map the orien- tity matrix.
tation distribution below four nanoindents of diﬀerent /ð2Þ À /ð1Þ ¼ ðD/ À IÞ/ð1Þ ð10Þ
depths. The experiment makes use of a tomographic
high-resolution electron backscatter diﬀraction orientation The orientation gradient, gij,k, is the orientation diﬀer-
microscope in conjunction with a focused ion beam instru- ence over the distance d between the two orientations,
ment for automated serial sectioning (3-D EBSD) . The Eq. (11). The minimum distance is in this study prescribed
GND densities are estimated below the four indents using by the EBSD step size.
EBSD data considering both the 2-D and the 3-D rota- /ð2Þij À /ð1Þij
tional gradients. gij;k ¼ ð11Þ
GNDs are characterized by two vectors, the Burgers vec-
2. Methods tor, b, representing the slip direction, and the normalized
tangent vector, ^, indicating the dislocation line direction.
Index notation is used: i.e. Aij denotes the components of a second-
The translation symmetry of the crystal lattice remains
order tensor; bold letters indicate vectors, b ¼ bi ^i where ^ is a Cartesian
intact during plastic deformation. The line integral of the unit vector; tensor products are represented as b t; the dot product of
displacement, dui, therefore, has to vanish around any area two vectors is t Á r=tiri.
E. Demir et al. / Acta Materialia 57 (2009) 559–569 561
Slip and line directions of dislocations for GNDs in a fcc crystal.
110 101 011 110
10 011 110 101 011
121 211 1
12 121 11
211 110 101 011
a Y b c ti
(sp 2D A
Z (111) g ij,2
 g ij,3
Fig. 1. (a) Focussed ion beam sectioning detail with relevant crystal directions. (b) Schematic illustration of the 2-D and 3-D analysis of the EBSD maps
obtained from the cross-sections.
There are 18 possible geometrical conﬁgurations of GNDs slice), are assumed to vanish, i.e. only the gradients in the
in fcc crystals (see Table 1). two in-plane directions are considered. In the 3-D analysis,
The orientation gradients can be related to GNDs with the full orientation gradients are estimated by the use of
the aid of a Frank’s loop construction around an area nor- additional orientation information from the neighboring
mal, r. This is also the vector around which the incompat- EBSD slices.
ibility is estimated, Eq. (5). The resulting net Burgers
vector, B, is the non-zero amount of dislocation lines pierc- 2.2. Experimental procedure
ing the area with the normal vector r, Eq. (12).
The copper single crystals were produced by directional
B ¼ bð^ Á rÞ ¼ ðb ^Þr
t t ð12Þ
solidiﬁcation in a Bridgeman furnace. The (111)-oriented
The Frank’s loop compensates the amount of incompat- surface was wet ground, diamond polished and electropo-
ibility that results from the measured orientation gradients, lished. The normal of the cross-section has a  crystal-
Eq. (13). However, an ambiguity exists when selecting 18 lographic direction (Z-direction in Fig. 1) [30,31].
scalar unknown densities (qa ) from the nine given compo-
gnd The indentation experiments were performed using a
nents of the dislocation tensor.2 In Eqs. (13) and (14), the Hysitron TriboScope indenter in load-controlled mode. A
superscript ‘‘a” represents the slip system. 60° conical indenter was used with a spherical tip of radius
18 R = 1 lm. A loading rate of 1.82 mN sÀ1 was used with
aij ¼ qa ba ta
gnd i j ð13Þ loads of 4000, 6000, 8000 and 10,000 lN producing four
a¼1 indents of diﬀerent depths. The corresponding depths are
A minimization method very similar to Taylor’s mini- 0.46, 0.69, 0.85 and 1.23 lm, respectively. The conical sur-
mum work approach  is used to identify nine unknown face (60° cone angle) of the indenter is in contact with the
dislocation densities that accommodate a given lattice cur- material at depths greater than half of the tool radius
vature (see details in Appendix A). (0.5 lm) during indentation. Therefore, the tool remains
self-similar during indentation only in case of the smallest
depth (0.46 lm).
aij ¼ qa ba ta
gnd i j ð14Þ
Fig. 2 shows the hardness values obtained for each indent.
The area function was determined using PMMA (polymeth-
The method is applied to both 2-D and 3-D tomo- ylmethacrylate) since the indentation depths were too large
graphic EBSD maps. In the 2-D analysis, the gradients to obtain a satisfactory calibration from fused quartz.
gij,3 along the sectioning direction (normal to each 2-D 3-D EBSD measurements of the deformed sample were
conducted using a dual-beam high-resolution ﬁeld emission
Note that the dislocation tensor is not necessarily a symmetrical tensor, scanning electron microscopy EBSD set-up together with a
hence it yields nine independent components. focused ion beam (FIB) system . The surface was
562 E. Demir et al. / Acta Materialia 57 (2009) 559–569
Fig. 2. Reduced elastic indentation modulus and indentation hardness values observed for the four diﬀerent indentation depths.
coated with Pt to avoid Ga+ damage during sectioning. size. On the other hand, a large step size shifts the anal-
Layers 100 nm thick were successively milled and EBSD ysis to a more mesoscopic level so that one might miss
measurements were carried out before each milling step the regime where strain gradients become eﬀective. In
[34,35]. The FIB milling procedure required for the tomo- addition, the small-scale nature of indentation prohibits
graphic EBSD method leads to minor edge eﬀects at the the use of a large step size approaching the depths of
surface. Therefore, we avoided probing very shallow the indents.
indents, i.e. the depths were chosen to assemble reliable The 2-D analysis explained in Section 2 is applied to the
EBSD data (more details are given in Refs. [30,31]). EBSD map obtained from the center cross-section using
three diﬀerent step sizes for comparison, i.e. 50, 100 and
2.3. EBSD data 200 nm (Fig. 4). A step size above 200 nm is not considered
since it approaches the depth of the indents ($400 nm for
Fig. 3 shows the orientation patterns in three diﬀerent the smallest indent). The step size used during EBSD data
slices that are equally spaced around the center position acquisition was 50 nm. The coarse graining of the data was
(section 39). The patterns before and after the center sec- performed using TSL software.3
tion are not symmetric with respect to the center of the The step size used for the gradient analysis inﬂuences the
indent. Section 33 (À600 nm from center layer) reveals distribution and the total magnitude of the GNDs. First, due
sharper orientation changes compared to section 45 to the averaging of neighboring orientations during coarse
(+600 nm from center layer). Also the magnitude of the graining, the GND density is locally averaged into larger vol-
orientation changes are slightly diﬀerent among the two umes. Second, higher orientation gradients occur in the case
outer sections. The diﬀerence in the texture evolution with of a larger step size (200 nm) when compared to those
respect to the sectioning direction is attributed to the crys- obtained in case of smaller step sizes. Higher orientation gra-
tallographic asymmetry of the orientation relative to dients mean higher magnitudes of GNDs. Third, some local
loading. peak information may be lost if a coarse step size is selected
due to averaging (200 nm in this case). For step sizes of 50
3. Experimental results and discussion and 100 nm, the peak values remain the same (3.5 Â
1016 mÀ2), indicating no loss of essential information. The
3.1. Selection of step size for the GND analysis gradient peak value drops to 2.4 Â 1016 mÀ2 for the
200 nm step size which indicates a peak smoothing eﬀect.
The selection of the gradient step size plays an However, the average overall GND density becomes larger
important role in establishing a reliable analysis for for this step size (Fig. 4).
the GND density (see dk in Eq. (11)). As the orienta-
tions are integrated and averaged over a larger region,
the noise in the data typically drops with increasing step TSL is a trademark of EDAX/TSL, Draper, UT.
E. Demir et al. / Acta Materialia 57 (2009) 559–569 563
Fig. 3. The orientation distribution below and around indents, the center section and two equally distant outer sections. Color code: crystal axis along the
direction of indentation.
3.2. 2-D GND analysis of ﬁve EBSD sections 3.3. 2-D GND analysis of all EBSD sections and comparison
to the hardness
First, the 2-D analysis is individually applied to ﬁve
equally spaced cross-sections, i.e. the center slice (section Fig. 8 shows the total 2-D GND density below each
39) and the two nearest sections on either side (±100 and indent together with the measured hardness values. The
±200 nm). The comparison of the four indents in the center total 2-D GND density is obtained by summing the GNDs
section is reasonable since the cone shape eﬀects are over all 50 individual 2-D EBSD sections and dividing this
expected to be minimum close to the center (Fig. 5). number by the total reference volume (Fig. 9). For this pur-
The sum of the GND densities beneath each indent was pose the GND density was ﬁrst calculated separately for
calculated by dividing their number by the aﬀected refer- each 2-D slice and subsequently the overall density was
ence volumes (see details in Appendix A). This normaliza- determined by summing over the 50 sections (see Appendix
tion step renders the GND dislocation number value a A). The data show that the GND density decreases with
density measure. The reference volumes were determined decreasing indentation depth and increasing hardness.
by using a threshold value for the GNDs. Fig. 6 shows a The density of the GNDs decreases faster with decreasing
corresponding example calculation containing the total indentation depth than the aﬀected reference volume. This
length of the GNDs beneath each indent. leads to an overall decrease in the GND density for smaller
Fig. 7 shows the sum of the GND densities below each indents.
indent that are extracted individually for each of the ﬁve 2-
D EBSD maps. The main observation is that the total 3.4. 3-D GND analysis
GND density decreases with decreasing depth and increas-
ing hardness of the indents (Figs. 2 and 7). The GND den- Five sections closest to the center are used for the calcu-
sity variation before and after the center section is lation of the GND densities considering also the out-of-
attributed to the asymmetry of deformation. The GND plane orientation gradients, gij,3 – 0 (Fig. 10). It has to
densities are larger in the front sections 37 and 38 com- be emphasized, however, that the full tomographic analysis
pared to the sections behind the center. requires the neighboring EBSD slices to be perfectly
564 E. Demir et al. / Acta Materialia 57 (2009) 559–569
Fig. 4. The distribution of the GND density below four indents in the center section for three diﬀerent step sizes: 50 nm (minimum step size as prescribed
by EBSD resolution), 100 and 200 nm (top to bottom). Color code: GND density in decadic logarithmic scale (mÀ2).
aligned with respect to each other to avoid artiﬁcial gradi- [30–33]. The third observation, however, contradicts the
ents due to misalignment. The results of the full 3-D anal- commonly expected inverse relationship between the inden-
ysis (see Fig. 10) are similar to those obtained from the tation depth and the density of the GNDs. The GND-based
accumulative 2-D analysis (Fig. 8). A slightly higher strain gradient theories that are usually applied to analyze
GND distribution is found underneath the indents in the indentation size eﬀects associate larger GND densities with
3-D analysis compared to the 2-D results. This is due to smaller indents but not with larger indents [15–17]. Our anal-
the small misalignment between the neighboring sections ysis shows the opposite trend. Of course these results are only
as discussed above. valid for the selected indentation depths and type of indenter
used. It must be noted in that context that depending on the
3.5. Relationship between GND density, indentation depth details of the indenter and tip geometry, the theoretically
and hardness expected GND density may in special cases also be indepen-
dent rather than inversely related to the indentation depth.
The results reveal three main points. Firstly, the GNDs However, a steep decay of the GND density for smaller
are not arranged homogeneously but in the form of pat- indents as found in this study was neither experimentally
terns below and around the indents. Secondly the distribu- observed nor theoretically predicted up to now.
tion of the GND density is anisotropic with respect to the Another aspect that deserves attention is the indentation
center slice. Thirdly, and most importantly, the density of size regime. The indents under investigation are between
the GNDs does not increase with decreasing indentation 1230 and 460 nm deep. The indentation size eﬀect is, how-
depth but rather drops. The GND density decreases from ever, more pronounced for shallower indents. For scales
%2.34 Â 1015 mÀ2 (largest indent) to %1.85 Â 1015 mÀ2 below 460 nm, however, the EBSD method would be of lim-
(smallest indent) while the hardness increases from ited help since it is has a lateral resolution of 40–50 nm in
%2.08 GPa for the largest indent (1230 nm) to %2.43 GPa copper [33,30,31]. Irrespective of the rather large size of the
for the smallest one (460 nm) (Fig. 8). indents and the comparably weak size eﬀect in this depth
The ﬁrst two observations, namely GND patterning and regime, the current observations document the occurrence
anisotropy of the lattice curvature, were reported before of an indentation size eﬀect (Figs. 2 and 8).
E. Demir et al. / Acta Materialia 57 (2009) 559–569 565
Fig. 5. Five equally spaced cross-sections (center slice, ±100 nm, ±200 nm) through the four indents. Color code: GND density in decadic logarithmic
scale (mÀ2). The noise level for the determination of the GND density is 1014 mÀ2 for a step size of 100 nm.
566 E. Demir et al. / Acta Materialia 57 (2009) 559–569
Fig. 6. Reference volumes (red color, e.g. center EBSD section) below the indents which indicate the zones that were aﬀected by the indent deformation.
The aﬀected volumes were determined by using a threshold value for the GNDs to render the dislocation number value a density measure. Color code:
GND density in decadic logarithmic scale (mÀ2).
-200nm -100nm 0nm (Center Sect.) 100nm 200nm
0.4 0.5 0.6 0.7 0.8 0.9 1 1.1 1.2 1.3
Fig. 7. Total GND densities that are extracted individually from each of the ﬁve 2-D EBSD maps that are closest to the center slice below the four indents.
The total GND density decreases with decreasing indentation depths.
This means that the GND density cannot in the current in turn is the main parameter for the activation of disloca-
case explain the indentation size eﬀect. An alternative tion sources in terms of the Frank–Read stress (the activa-
explanation could be that the SSDs are responsible for tion stress for a dislocation source is inversely proportional
the increase in hardness at small scales. This explanation to the dislocation segment length). For small indents the
is, however, also not plausible since the density of the SSDs interface-to-volume ratio is higher compared to large ones.
is linked to the strain and in the current case the total strain Assuming a rapid drop in the free dislocation segment
decreases with decreasing indentation depth. Another length in these narrow contact zones, therefore, might
explanation might be a dislocation source limitation eﬀect. qualitatively explain why smaller indents yield a higher
Conventional dislocation multiplication and hardening hardness than large ones. The reason, however, would
may be expected to be highly localized close to the contact not be a larger density of GNDs alone but their contribu-
zone between indenter and specimen. The increase in the tion to the reduction in the free dislocation segment length.
overall dislocation density (including GNDs) leads to a According to this approach, the mechanical size eﬀect
rapid drop in the free dislocation segment length, which observed in this work would not be due to the hardening
E. Demir et al. / Acta Materialia 57 (2009) 559–569 567
Fig. 8. The total GND densities below each indent obtained by summation over all 50 individual 2-D EBSD sections together with the measured hardness.
Fig. 9. 3-D view of the volume around the four indents. Upper row: EBSD pattern quality. The bright gray scale indicates large local lattice distortions.
Bottom row: local orientation deviation. The color code is chosen to indicate the largest local orientation changes (15°) in red.
contribution of the GNDs but due to a dislocation multi- Cu single crystal using a conical indenter with spherical
plication limitation eﬀect. This idea of source strengthening tip of radius 1 lm. The deformation-induced lattice rota-
in conjunction with the indentation size eﬀects has also tions were monitored using a tomographic EBSD method.
been discussed by Pippan et al. . The GND densities were calculated from the measured
rotations using the dislocation density tensor which con-
4. Conclusions nects lattice curvature to GNDs. This approach allowed
us to directly quantify in one experiment both the mechan-
We studied the eﬀect of the indentation size eﬀect and ical parameters (depth, hardness) and the lattice defects
the GND density by using the following approach. Four (GNDs) that are held responsible for the indentation size
indents of diﬀerent depth and hardness were placed in a eﬀect. The main results are:
568 E. Demir et al. / Acta Materialia 57 (2009) 559–569
-200nm -100nm 0nm (Center Sect.) 100nm 200nm
0.4 0.5 0.6 0.7 0.8 0.9 1 1.1 1.2 1.3
Fig. 10. GND densities calculated considering the gradients also in the third direction (perpendicular to the slices) for the ﬁve central slices closest to the
The GNDs have an inhomogeneous distribution under- mat) is processed to identify a GND density for every data
neath the indents with very high local density values. point. The solution procedure uses ﬁve steps: (i) Nine slip
This fact questions the homogeneous distribution systems (corresponding to the nine components of the dis-
assumptions frequently used in the literature. location density tensor) are selected arbitrarily from the 18
The heterogeneous distribution in GND density might possible GND systems (48,620 possible combinations). (ii)
play the key role in strengthening since a long-range The slip system combinations are checked for geometrical
back stress ﬁeld develops due to imbalance in signed dis- independence and 21,464 linearly independent solutions
location density and resists dislocation motion. are found. (iii) A solution is calculated for each possible
The total GND density below the indents decreases with combination of nine slip systems. (iv) The total GND den-
decreasing indentation depth. This observation contra- sity, which is the sum of the absolute values of the nine
dicts the strain gradient theories attributing size-depen- individual GND densities, is calculated. (v) The solution
dent material properties to GNDs. yielding the minimum total GND density among all possi-
The amount of deformation imposed reduces with ble combinations is selected.
decreasing indentation depth. Therefore, SSDs that There are three main input quantities to the analysis,
evolve through strain do not account for the increasing i.e. the Burgers vector, the gradient step sizes in the x, y
hardness values with decreasing indentation depth. and z directions, and the lower threshold limit for the
The decreasing dislocation segment lengths associated misorientations. The Burgers vector is 2.5 Â 10À4 lm in
with decreasing indentation depth are believed to the case of copper. The inﬂuence of the step size used
account for the increase in hardness. for the gradient calculation has been discussed in Section
Explaining size-dependent material strengthening eﬀects by 3.1. A lower limit for misorientations is used to eliminate
using average density measures for both GNDs and SSDs noise and to save analysis time. On the contrary, some
is not suﬃcient to understand the indentation size eﬀect. information may be lost depending on the value of the
lower limit. Therefore, the lower limit is selected slightly
above the noise level (0.5°) so that a minimum amount
Acknowledgements of information is lost.
The GNDs have to be summed over the deformed
We thank Dr. F. Roters for his valuable contribution to region in order to identify the total GND density under
the calculation of gradients. Comments of Dr. Y. Cao on an indent. The total GND density is estimated by summing
data interpretation are greatly appreciated. One of the the number of all GNDs and dividing this value by the
authors (E.D.) also acknowledges the lectures of Prof. total reference volume (Fig. 6). Firstly, the region aﬀected
A.D. Rollett at Carnegie Mellon University. by an indent is selected. Secondly, the densities of each
point that exceeds the lower bound are summed and the
Appendix A. Details of the analysis of GNDs from EBSD total number of all data points are counted. Finally, the
data total density of the region is found by dividing the sum
of the GND densities by the number of points, Eq. (15).
The procedure to extract GNDs from EBSD data was (In Eq. (15), N represents the number of points and A0
implemented in MatLab. The EBSD output ﬁle (TSL for- stands for the unit area aﬀected.)
E. Demir et al. / Acta Materialia 57 (2009) 559–569 569
iq A0 iq
 Gao H, Huang Y, Nix WD. Naturwissenschaftler 1999;86:
gnd ¼ P gnd ¼ P gnd ð15Þ 507–15.
i N i A0 iN
 Gao H, Huang Y. Scripta Mater 2003;48:113–8.
 Motz C, Schoberl T, Pippan R. Acta Mater 2005;53:4269–79.
 Trivedi PB, Yassar RS, Field DP, Alldredge R. Mater Sci Eng
 Acharya A, Basani JL. J Mech Phys Sol 2000;48:1565–95.
 Uchic MD, Dimiduk DM, Florando JN, Nix WD. Science  Arsenlis A, Parks DM. Acta Mater 1999;47:1597–611.
2004;305:986–9.  Sun S, Adams BL, King WE. Philos Mag 2000;80:9–25.
 Greer JR, Oliver WC, Nix WD. Acta Mater 2005;53:1821–30.  El-Dasher BS, Adams BL, Rollett AD. Scripta Mater
 Nix WD, Greer JR, Feng G, Lilleodden ET. Thin Solid Films 2003;48:141–5.
2007;515:3152–7.  Field DP, Trivedi PB, Wright SI, Kumar M. Ultramicroscopy
 Dehm G, Motz C, Scheu C, Clemens H, Mayrhofer H, Mitterer C. 2005;103:33–9.
Adv Eng Mater 2006;8:1033–45.  Brewer LN, Othon MA, Young LM, Angeliu TM. Microsc Micro-
 Nye JF. Acta Metall 1953;1:153–62. anal 2006;12:85–91.
 Bilby BA, Gardner RT, Smith E. Acta Metall 1958;6:29–33.  Field DP, Merriman CC, Smith JM. Microsc Microanal
 Kroner E. Int J Eng Sci 1963;1:261–78.
 Ashby MF. Philos Mag 1970;21:399–424.  Kubin LP, Mortensen A. Scripta Mater 2003;48:119–25.
 Kocks UF. Philos Mag 1996;13:541–66.  Taylor GI. Inst Metals 1938;62:307–25.
 Roters F, Raabe D, Gottstein G. Acta Mater 2000;48:4181–9.  Zaafarani N, Raabe D, Singh RN, Roters F, Zaeﬀerer S. Acta Mater
 Begley MR, Hutchinson JW. J Mech Phys Sol 1998;46:2049–68. 2006;54:1863–76.
 Gerberich WW, Tymiak NI, Grunlan JC, Horstemeyer MF, Baskes  Zaafarani N, Raabe D, Roters F, Zaeﬀerer S. Acta Mater
MI. J Appl Mech 2002;69:433–42. 2008;56:31–42.
 Trivedi PB, Yassar RS, Field DP, Alldredge R. Mater Sci Eng  Rester M, Motz C, Pippan R. Acta Mater 2007;55:6427–35.
2006;434:178–87.  Zaeﬀerer S, Wright SI, Raabe DS. Metall Mater Trans A
 Brinckmann S, Siegmund T, Huang Y. Int J Plast 2006;22:1784–97. 2008;39A:374–89.
 Fleck NA, Muller GM, Ashby MF, Hutchinson JW. Acta Metall  Konrad J, Zaeﬀerer S, Raabe D. Acta Mater 2006;54:1369–80.
1994;42:475–87.  Bastos A, Zaeﬀerer S, Raabe D. J Microsc 2008;230:487–98.
 Nix WD, Gao H. J Mech Phys Sol 1998;46:411–25.